Abstract
Since its invention, holography has emerged as a powerful tool to fully reconstruct the wavefronts of light including all the fundamental properties (amplitude, phase, polarization, wave vector, and frequency). For exploring the full capability for information storage/display and enhancing the encryption security of metasurface holograms, smart multiplexing techniques together with suitable metasurface designs are highly demanded. Here, we integrate multiple polarization manipulation channels for various spatial phase profiles into a single birefringent vectorial hologram by completely avoiding unwanted crosstalk. Multiple independent target phase profiles with quantified phase relations that can process significantly different information in different polarization states are realized within a single metasurface. For our metasurface holograms, we demonstrate high fidelity, large efficiency, broadband operation, and a total of twelve polarization channels. Such multichannel polarization multiplexing can be used for dynamic vectorial holographic display and can provide triple protection for optical security. The concept is appealing for applications of arbitrary spin to angular momentum conversion and various phase modulation/beam shaping elements.
Introduction
Holography based on metasurfaces has emerged as a promising candidate for applications in optical displays, optical storage and security by exhibiting unprecedented spatial resolution, enormous information capacity and a large field of view compared to traditional methods^{1,2,3,4,5,6,7,8,9,10,11}. The practical realization of metasurface holograms relies on the encoding of holographic profiles on ultrathin nanostructures, which can possess strong lightmatter interaction within an ultrashort distance^{12,13,14,15,16,17,18}. Many efforts have been put into incorporating novel holographicrelated functionalities such as beam shaping and ghost imaging into metasurfaces^{19,20,21,22}. By utilizing the arbitrary design freedom of metasurfaces to simultaneously engineer the local wavelength, amplitude, phase, and polarization response, it might be possible to provide a flexible and compact platform to realize all types of vectorial holograms (with highdimensional information) rather than scalar intensity information, which can surpass the limitations of natural materials such as liquid crystals or optical photoresists^{23,24,25,26}.
For the purpose of optimizing the tremendous information capability of metasurface holograms, multiplexing techniques are highly desired including color holograms^{27,28,29}, polarization multiplexing^{30,31,32,33,34} and hybrid multiplexing^{35,36}. Among the mentioned multiplexing techniques, polarization multiplexing is an attractive method due to polarization sensitivity of artificially tailored metaatoms that can completely alter the polarization state of the interacting light. Polarization multiplexed metasurface holograms that support only two orthogonal states and based on spatial multiplexing with more than one metaatom within a unitcell have been described previously^{30,31}. Such spatial multiplexing usually results in strong crosstalk between the information channels and lowers the spacebandwidth product. Furthermore, the increased space requirement for the larger unit cell reduces the information density, which might counterbalance the additional information capacity of the second polarization channel. By using birefringent metasurfaces composed of a single metaatom per unitcell that possess a variation in the phase shifts for the orthogonal polarization states, an alternative approach for realizing polarization multiplexing has been demonstrated^{32,33}. Nevertheless, the full capacity of all polarization channels (input/output polarizations) has not yet been explored. This limits the improvement of the information capacity stored in metasurface holograms and restricts the versatile functionality of holographicbased optical devices.
Here, we demonstrate a novel method for realizing multichannel vectorial holography and show its potential for obtaining dynamic displays and highsecurity applications. We explore birefringent metasurfaces for the complete control of polarization channels with the freedom of designing both the polarizationdependent phase shift and polarization rotation matrix. We show that although the target holographic phase profiles have quantified phase relations, they can process very different information within different polarization manipulation channels. The reconstructed vectorial images can be switched with negligible crosstalk by selecting the desired combination of input/output polarization states. A set of reconstructed images can conceive different meanings and therefore host unique merits for encryption. Our demonstrated multiplexing method may lead to a new frontier for applications related to dynamic holographic displays, switchable optical devices, data storage, and optical encryption/anticounterfeiting, which are compatible with most optical systems that operate in transmission. Furthermore, our proposed method can also be adapted to arbitrary spin to orbital angular momentum conversion or other types of polarization/phase modulation and enhance the information capacity.
Results
We comparatively study two schemes of multiple polarization channels (from orthogonal two channels to twelve channels) by using birefringent dielectric metasurfaces, as shown in Fig. 1. We show that polarization and anglemultiplexed holograms can be realized by utilizing nanofins with different crosssections but without rotation (Fig. 1a). Two sets of offaxis holographic images can be generated with two orthogonal states. However, by considering the flexibility for designing the entire Jones matrix, we can achieve more multiplexed functionalities with complete control of polarization and phase (Fig. 1b). Three independent images (we chose the words “holography”, “meta”, and “surface” as the reconstructed images) can be reconstructed successfully with high resolution and high fidelity for different combinations of input and output polarization channels. All combinations of thse three images in a total of twelve different polarization channels can be observed (“meta” + “holography”, “meta” + “surface”, “surface” + “holography” and “meta” + “surface” + “holography”) with satisfactory efficiencies. In addition, the reconstructed images exhibit a vectorial feature for the polarization state of the different words in analogy to optical vector beams.
For achieving multichannel vectorial holography, we have to explore suitable building blocks for the metasurfaces. As is well known, the general relation between the electric field of the input (E^{in}) and output (E^{out}) waves at each pixel can be expressed using the Jones matrix description:
Indeed, any desired symmetric and unitary Jones matrix can be realized using a birefringent metasurface if the polarizationdependent phase shift (ϕ_{x}, ϕ_{y}) and the orientation angle θ can be chosen freely^{33}:
where Δ indicates the eigenvalue matrix of the Jones matrix T and the real unitary matrix V can be treated as a rotation matrix R. Crucially, the desired phases (combining both dynamic and geometric phases) can be extended to impart on any set of orthogonal polarization states.
We first consider the twochannel polarization multiplexed holograms as the simplest case. By formulating the Jones matrix of each pixel as:
We can easily tailor the desired output light to \(E_{x,{\kern 1pt} {\mathrm {inc}}}^{\mathrm {out}} = \left[ {\begin{array}{*{20}{c}} {e^{i\varphi _1}} \\ 0 \end{array}} \right]\) in each pixel according to the profile of the hologram 1 while guaranteeing the phase distribution of \(E_{y,{\kern 1pt} {\mathrm {inc}}}^{\mathrm {out}} = \left[ {\begin{array}{*{20}{c}} 0 \\ {e^{i\varphi _2}} \end{array}} \right]\). Therefore, the original image 1 and image 2 for orthogonal incident polarizations can be reconstructed and switched. These two channels for polarization multiplexed metasurface holograms can be easily realized by generating a polarizationdependent phase shift in the x and y directions but with an identical orientation angle for all nanofins. Note that to further enlarge the information capacity, one can also encode angular or distance multiplexed holographic images for each phase profile of φ_{1} and φ_{2}.
More complex multiplexed functionalities can be realized by utilizing the design freedom of the rotation matrix R. Assuming that the Jones vector of the output light is described by \(E_{x,{\kern 1pt} {\mathrm {inc}}}^{\mathrm {out}} = \frac{{\sqrt 2 }}{2}\left[ {\begin{array}{*{20}{c}} {e^{i\varphi _1}} \\ {e^{i\varphi _2}} \end{array}} \right]\) when the incident light is xpolarized light. Now, the x and y components of the output light can be designed to reconstruct the original holographic image 1 and image 2 with equal intensity and high contrast, respectively. More importantly, the reconstructed images can be switched by selecting the desired transmission polarization with negligible polarization crosstalk. For such a situation, the Jones matrix of each pixel can be derived as:
From the above Jones matrix, one can recognize that when the incident light polarization is changed to ypolarized light, the Jones vector of the output light will be expressed by \(E_{y,{\kern 1pt} {\mathrm {inc}}}^{\mathrm {out}} = \frac{{\sqrt 2 }}{2}\left[ {\begin{array}{*{20}{c}} {e^{i\varphi _2}} \\ {e^{i(2\varphi _2  \varphi _1 + \pi )}} \end{array}} \right]\). This additional phase relation between φ_{1} and φ_{2} for the ycomponent of the output field opens up the possibility of encoding an additional holographic image. By utilizing a suitable algorithm for the generation of holograms, holographic image 3 can be reconstructed by satisfying the relation φ_{3} = 2 × φ_{2} − φ_{1} + π. Hence, the ycomponent of the output light results in reconstruction of image 3 by illumination with ypolarized light. Meanwhile, the concept can be extended further by utilizing circular polarization states for the incident wave. For circularly polarized input light, the output field can be derived as:
where the super/subscript in the brackets denote the alternative case for orthogonal lefthandedness (L) or righthandedness (R) circular polarization. Based on the phase relation of the output fields, one can find that three different independent images (1–3) and all combinations of these images (1 + 2, 1 + 3, 2 + 3, 1 + 2 + 3) can be reconstructed from each item using the above equations, while a constant phase difference of ±π/2 and 0/π in Eq. 5 will only result in the same image. Hence, we obtain 12 channels in total (different combinations of incident/output polarization: T_{xx}, T_{xy}, T_{yx}, T_{yy}, T_{ll}, T_{lr}, T_{rl}, T_{rr}, E_{x}^{out}, E_{y}^{out}, E_{L}^{out}, E_{R}^{out}) and seven combinations of holographic images within one single metasurface, without any additional spatial multiplexing.
To acquire the target phase profiles to fulfill Eq. 4 (we can view Eq. 3 as a special case without rotation), both the hologram generation algorithm and suitable design of the metaatoms are key points. We build a new hologram algorithm based on a modified Gerchberg–Saxton (GS) scheme by considering the quantified relations of each other (φ_{1}, φ_{2,} and φ_{3} = 2φ_{2} − φ_{1} + π) to adapt to each polarization channel. As a phase retrieval method, the desired phase distribution obtained with the GS algorithm is calculated by constructing an iterative loop between the object plane and the hologram via a Fourier transform^{37}. Crucially, the phase φ_{3} has a quantified relation with both other phases φ_{1} and φ_{2}, while the latter two phase profiles can be altered independently. Therefore, we used another serial loop by connecting all of these three phase profiles. A flowchart with details can be found in the Supplementary Material. Meanwhile, we use the birefringence as well as the rotational property (adapted from Eq. 2) of the simplest rectangular nanofins with a tailorable crosssection and azimuthal angles. Such structures provide a suitable platform for the realization of multichannel vectorial holograms. To realize the desired phase shifts in each polarization channel, one has to guarantee that the phase shift of either φ_{1} or φ_{2} can cover the entire 0–2π range while still allowing all possible combinations of (φ_{1}, φ_{2}). Furthermore, we have to maintain a uniform amplitude distribution with high efficiency. A 2D parameter optimization by using a rigorous coupled wave analysis (RCWA) method was carried out. The simulation results for the amplitude and phase distribution of Si nanofin for the orthogonal polarization state illumination are shown in Fig. 2 (see Methods).
In the following, we fabricated several designed dielectric silicon metasurfaces on top of a glass substrate by using a plasma etching process, followed by electron beam lithography for patterning (see Methods). The experimental setup and two typical scanning electron microscopy images of the samples with and without rotation are shown in Fig. 3. For the specific simple case of no rotation (Eq. 3), we encode four separate original images into φ_{1} and φ_{2} by considering polarization and angular multiplexing, respectively, as shown in Fig. 4. This metasurface yields offaxis holographic images of a cartoon tiger and a snowman with high fidelity and high resolution when illuminated by xpolarized light. By switching to y polarization for the incident light, the reconstructed images are changed to a teapot and a cup. Note that in this case, there are only two polarization channels, with both pairs of the holographic image reconstructed and made to disappear simultaneously by rotating the polarizer behind the sample. For the polarization of the incident light with an angle of 45° or 135°, all four original images can be observed simultaneously. The experimental results are in good agreement with the simulation results, which confirms the basic design principle. In our experiment, we define two types of diffraction efficiencies. The diffraction efficiency of each polarization channel (T_{xx}, T_{xy}, T_{yx}, and T_{yy}) is defined as the ratio of the power of the output light in the different channels to the power of the incident light. These diffraction efficiencies of our fabricated samples are retrieved from spectral analysis (transmission spectra). The corresponding experimental results are shown in the Supplementary Material. The net diffraction efficiency for the holography is defined as the ratio of the intensity of the single reconstructed image to the power of the incident light (the residual power in the central area is not included). For the four reconstructed images, the net diffraction efficiencies (cartoon tiger, snowman, teapot, cup) are 15.37%, 10.87%, 13.08%, 10.92%, respectively (see the video and further efficiency analysis in the Supplementary Materials).
Furthermore, we fabricate another dielectric metasurface hologram that can utilize additional polarization channels by considering the additional design freedom afforded by the orientation angles of the nanofins. In such a way, more complex multiplexing functionalities can be obtained. From the linear polarization experimental results (top two rows), we observe that when the incident light is xpolarized, the x (\(E_{x,\;{\kern 1pt} {\mathrm {inc}}}^{x,\;{\kern 1pt} {\mathrm {out}}}\)) and y (\(E_{x,{\kern 1pt} {\mathrm {inc}}}^{y,{\kern 1pt} {\mathrm {out}}}\)) components of the output field will contribute to the reconstruction of the words “holography” and “meta”, respectively. Hence, the total electromagnetic field of the output light (\(E_{x,{\kern 1pt} {\mathrm {inc}}}^{{\mathrm {norm}},{\kern 1pt} {\mathrm {out}}}\)) results in reconstruction of both words (“holography” and “meta”) simultaneously, but with orthogonal ‘vectorial’ properties for each word (Fig. 5g–i). Upon switching to the incident light with y polarization, the x (\(E_{y,{\kern 1pt} {\mathrm {inc}}}^{x,{\kern 1pt} {\mathrm {out}}}\)) and y (\(E_{y,{\kern 1pt} {\mathrm {inc}}}^{y,{\kern 1pt} {\mathrm {out}}}\)) components of the output light will be switched to reconstruct the words “meta” and “surface”, respectively (Fig. 5j–l). We further carried out verification of the multiplexed holograms under illumination with circularly polarized light (bottom two rows). When the incident light is LCP/RCP, we can observe the words “holography” and “surface” simultaneously by selecting the LCP (\(E_{L,{\kern 1pt} inc}^{L,{\kern 1pt} out}\))/RCP (\(E_{R,\;{\kern 1pt} {\mathrm {inc}}}^{R,\;{\kern 1pt} {\mathrm {out}}}\)) components of the output light (Fig. 5w, s). All three images can be obtained by using the RCP (\(E_{L,{\kern 1pt} inc}^{R,{\kern 1pt} out}\))/LCP (\(E_{R,\; {\mathrm {inc}}}^{L,\; {\mathrm {out}}}\)) components of the output light (Fig. 5v, t). Similarly, we can determine that the vectorial nature of the reconstructed images of the words “holography” and “surface” is linearly polarized from Eq. 5. While for the word “meta”, it only appears in the orthogonal circular polarization channels (Fig. 5x, u), as can be derived from Eq. 5. Therefore, the polarization state of the reconstructed word “meta” is right (left) handedness circularly polarized. Further analysis of arbitrary elliptical input/output polarization combinations can be carried out that will result in a much more complex “vectorial” nature for the reconstructed holographic images. We determined the net diffraction efficiencies for the reconstructed images (“holography”, “meta”, and “surface”) to be 15.97%, 8.03%, and 9.91% for the case of a linearly polarized combination, respectively. Therefore, three independent images and all the combinations of these images (12 channels in total with seven different combinations) can be reconstructed with high contrast by our proposed method. Additional results for demonstrating the feasibility of achieving a dynamic holographic display and efficiency analysis can be found in the Supplementary Material.
In addition, the method also enables encrypting different original images that can be superimposed at the same spatial location. Such superposition has the ability to convey a different meaning in the reconstructed image and can be used to provide alterable information content for the image, i.e., encryption, as shown in Fig. 6. Here, we chose a dice as our original image. The dice has six faces that are represented by the number of pips on the surface. Interestingly, by using a suitable selection of different combinations of input/output polarization states, a different number of pips (from one to six) can be observed. This kind of illusion for viewing different sides of the dice results from the increased multiplexing capability of our method that can encode up to six different images for the various combinations of polarization states (see the video in the Supplementary Materials).
Discussion
Our demonstrated multiplexing algorithm can result in a dynamic vectorial holographic display and encryption. Only by using the correct polarization keys can the receiver obtain the exact information delivered (as for the dice case). An even higher flexibility can be obtained by further increasing the complexity of the images (for example, by using more than two dice as the original images or using angle/distance/hybrid multiplexing in each independent phase profile) together with a detailed analysis of the reconstructed vectorial image properties. Such a metasurface with a compact physical size is easy to hide and transport. Even if the metasurface eavesdrops, the correct polarization combination (input/output) together with the additional vectorial nature of each image can provide a triple protection security lock for the communication information, which will greatly enhance the complexity of the decryption.
Such multichannel vectorial holography also exhibits a relatively large working bandwidth. This phenomenon can be understood in the following manner: due to the robustness of our silicon metasurface holograms and the fact that holograms generated by the GS algorithm are wavelength independent, together with the small variation of the Si refractive index, the reconstructed images can be observed with high fidelity even away from our design wavelength of 800 nm by using dielectric metasurfaces. In our experiment, we can achieve broadband reconstruction from the nearinfrared region to visible light (between 600 nm and 800 nm) with or without rotation of the nanofins. Detailed analysis through consideration of the phase shift caused by different wavelengths and statistics number for each nanofin over the entire metasurfaces together with reconstruction of the Jones matrix to accurately predict the broadband effect from simulation and experimental verification can be found in the Supplementary Material. Such a phenomenon can demonstrate the robustness of the metasurface holograms and can be further applied to realize color images. Alternatively, Titanium Dioxide (TiO_{2}) or Silicon Nitride (SiN) can be used to realize such holograms in the visible range with larger efficiency.
Information and image multiplexing based on the polarization states of light is a powerful tool that can be easily realized with optical metasurfaces. Here, we have demonstrated a novel method for achieving multichannel vectorial holography based on birefringent alldielectric metasurfaces to explore the full capacity of polarization. By considering the birefringent anisotropy property and extra design freedom afforded by the rotation matrix, together with the use of smart multiplexing algorithms for establishing quantified related phase profiles, highdimensional multichannel polarization multiplexed holograms were successfully realized using a simple nanofin as the building block. Compared to previously demonstrated metasurface multiplexed holograms that can only be switched between two states by incident light with two orthogonal polarization states, here, all combinations within twelve polarization channels in total can be obtained. Further application of arbitrary spin to angular momentum conversion and various phase modulation/beam shaping can be realized accordingly.
Materials and methods
Fabrication of the metasurfaces
The dielectric metasurfaces were fabricated on a glass substrate following the processes of deposition, patterning, lift off and etching. First, a 600nmthick amorphous silicon (aSi) film was deposited by plasma enhanced chemical vapor deposition (PECVD). A polymethylmethacrylate resist layer was spincoated onto the aSi film and baked on a hot plate at 180 °C for 2 min to remove the solvent. Then, the desired structure was patterned by using standard electron beam lithography and subsequent development in 1:3 MIBK:IPA solution. Next, the sample was washed with IPA before being coated with a 45nmthick chromium layer by electron beam evaporation. Next, a liftoff process in hot acetone was performed. Finally, by using inductively coupled plasma reactive ion etching (ICPRIE), the desired structure was transferred from chromium to silicon. The metasurfaces are composed of 1000 × 1000 nanofins (lattice constant along the x and yaxis of 400 nm) with different crosssections (width and length in the range of 80–280 nm, height 600 nm) and orientation angles. To minimize fabrication errors and to obtain highquality nanostructures, we took several precautions. Before fabricating the actual metasurface with all the various types of nanopillars, we first optimized the nanopillars with the smallest size (with and without rotation) for the electron beam lithography and the plasma etching process. After the best parameters were obtained for each nanopillar size, we used these values for the fabrication of the actual metasurface sample. We found that the structure size deviation is below 5% compared to the target values.
Design and numerical simulations
Our birefringent dielectric metasurfaces are designed using amorphous silicon nanofins on top of a glass substrate, as shown in Fig. 2a. To achieve the desired phase shifts (φ_{x}, φ_{y}), we carry out a 2D parameter optimization by using a rigorous coupled wave analysis (RCWA) method. The length L and width W of the nanofin are both swept in the range of 80–280 nm, while maintaining the height H at 600 nm and the period size P at 400 nm. The values for H and S are carefully chosen to guarantee that the phase of the output light can cover 0–2π and eliminate undesired orders of diffraction. For the simulation, the nanofin is placed onto a glass substrate (n_{SiO2} = 1.5). The wavelength of incident light is fixed at 800 nm, and the corresponding refractive index of amorphous silicon is n_{Si} = 3.6941 + 0.0065435*1i. The obtained transmission amplitudes and phases for the two transmission coefficients t_{xx} and t_{yy} are shown in Fig. 2b–d. We found that the transmission amplitudes for most of the nanofins with different crosssections are over 90%. Note that the orientation angles of the nanofins are determined by Eqs. 2 and 4 for the multichannel polarization multiplexing.
Optical measurement
For the optical characterization of the performance of the metasurface holograms, we use the setup that is shown in Fig. 3. A pair of linear polarizers or a combination of linear polarizers and quarterwave plates is placed in front of and behind the sample to select the desired incident/transmitted linearly/circularly polarized beam. Our metasurface sample is placed in the focal plane of an objective lens (×40/NA = 0.6) to guarantee that the Fourier plane is located in the back focal plane. Meanwhile, the magnifying ratio and numerical aperture of the objective lens are carefully chosen for the purpose of collecting all the diffraction light from the sample and reconstructing the holographic images in the Fourier plane. Another objective/lens is used for capturing the Fourier plane on a CCD camera.
References
Zheng, G. X. et al. Metasurface holograms reaching 80% efficiency. Nat. Nanotechnol. 10, 308–312 (2015).
Khorasaninejad, M., Ambrosio, A., Kanhaiya, P. & Capasso, F. Broadband and chiral binary dielectric metaholograms. Sci. Adv. 2, e1501258 (2016).
Devlin, R. C., Khorasaninejad, M., Chen, W. T., Oh, J. & Capasso, F. Broadband highefficiency dielectric metasurfaces for the visible spectrum. Proc. Natl Acad. Sci. USA 113, 10473–10478 (2016).
Ni, X. J., Kildishev, A. V. & Shalaev, V. M. Metasurface holograms for visible light. Nat. Commun. 4, 2807 (2013).
Wang, L. et al. Grayscale transparent metasurface holograms. Optica 3, 1504–1505 (2016).
Lee, G. Y. et al. Complete amplitude and phase control of light using broadband holographic metasurfaces. Nanoscale 10, 4237–4245 (2018).
Xiao, S. Y., Zhong, F., Liu, H., Zhu, S. N. & Li, J. Flexible coherent control of plasmonic spinhall effect. Nat. Commun. 6, 8360 (2015).
Xu, Q. et al. Polarizationcontrolled surface plasmon holography. Laser Photonics Rev. 11, 1600212 (2017).
Huang, L. L. et al. Threedimensional optical holography using a plasmonic metasurface. Nat. Commun. 4, 2808 (2013).
Zhang, C. M. et al. Multichannel metasurface for simultaneous control of holograms and twisted light beams. ACS Photonics 4, 1906–1912 (2017).
Yue, F. Y. et al. Multichannel polarizationcontrollable superpositions of orbital angular momentum states. Adv. Mater. 29, 1603838 (2017).
Kildishev, A. V., Boltasseva, A. & Shalaev, V. M. Planar photonics with metasurfaces. Science 339, 1232009 (2013).
Yu, N. F. & Capasso, F. Flat optics with designer metasurfaces. Nat. Mater. 13, 139–150 (2014).
Yu, N. F. et al. Light propagation with phase discontinuities: generalized laws of reflection and refraction. Science 334, 333–337 (2011).
Jahani, S. & Jacob, Z. Alldielectric metamaterials. Nat. Nanotechnol. 11, 23–36 (2016).
Lin, D. M., Fan, P. Y., Hasman, E. & Brongersma, M. L. Dielectric gradient metasurface optical elements. Science 345, 298–302 (2014).
Kuznetsov, A. I., Miroshnichenko, A. E., Brongersma, M. L., Kivshar, Y. S. & Luk’yanchuk, B. Optically resonant dielectric nanostructures. Science 354, aag2472 (2016).
Zheludev, N. I. & Kivshar, Y. S. From metamaterials to metadevices. Nat. Mater. 11, 917–924 (2012).
Genevet, P., Lin, J., Kats, M. A. & Capasso, F. Holographic detection of the orbital angular momentum of light with plasmonic photodiodes. Nat. Commun. 3, 1278 (2012).
Lin, J., Genevet, P., Kats, M. A., Antoniou, N. & Capasso, F. Nanostructured holograms for broadband manipulation of vector beams. Nano. Lett. 13, 4269–4274 (2013).
Epstein, I., Lilach, Y. & Arie, A. Shaping plasmonic light beams with nearfield plasmonic holograms. J. Opt. Soc. Am. B 31, 1642–1647 (2014).
Liu, H. C. et al. Singlepixel computational ghost imaging with helicitydependent metasurface hologram. Sci. Adv. 3, e1701477 (2017).
Gabor, D. A new microscopic principle. Nature 161, 777–778 (1948).
Leith, E. N. & Upatnieks, J. Reconstructed wavefronts and communication theory. J. Opt. Soc. Am. 52, 1123–1130 (1962).
Genevet, P. & Capasso, F. Holographic optical metasurfaces: a review of current progress. Rep. Prog. Phys. 78, 024401 (2015).
Huang, L. L., Zhang, S. & Zentgraf, T. Metasurface holography: from fundamentals to applications. Nanophotonics 7, 1169–1190 (2018).
Wang, B. et al. Visiblefrequency dielectric metasurfaces for multiwavelength achromatic and highly dispersive holograms. Nano. Lett. 16, 5235–5240 (2016).
Wang, B. et al. Polarizationcontrolled colortunable holograms with dielectric metasurfaces. Optica 4, 1368–1371 (2017).
Huang, Y. W. et al. Aluminum plasmonic multicolor metahologram. Nano. Lett. 15, 3122–3127 (2015).
Montelongo, Y., TenorioPearl, J. O., Milne, W. I. & Wilkinson, T. D. Polarization switchable diffraction based on subwavelength plasmonic nanoantennas. Nano. Lett. 14, 294–298 (2014).
Wen, D. D. et al. Helicity multiplexed broadband metasurface holograms. Nat. Commun. 6, 8241 (2015).
Mueller, J. P. B., Rubin, N. A., Devlin, R. C., Groever, B. & Capasso, F. Metasurface polarization optics: independent phase control of arbitrary orthogonal states of polarization. Phys. Rev. Lett. 118, 113901 (2017).
Arbabi, A., Horie, Y., Bagheri, M. & Faraon, A. Dielectric metasurfaces for complete control of phase and polarization with subwavelength spatial resolution and high transmission. Nat. Nanotechnol. 10, 937–943 (2015).
Chen, W. T. et al. Highefficiency broadband metahologram with polarizationcontrolled dual images. Nano. Lett. 14, 225–230 (2014).
Huang, L. L. et al. Broadband hybrid holographic multiplexing with geometric metasurfaces. Adv. Mater. 27, 6444–6449 (2015).
Ye, W. M. et al. Spin and wavelength multiplexed nonlinear metasurface holography. Nat. Commun. 7, 11930 (2016).
Wei, Q. S., Huang, L. L., Li, X. W., Liu, J. & Wang, Y. T. Broadband multiplane holography based on plasmonic metasurface. Adv. Opt. Mater. 5, 1700434 (2017).
Acknowledgements
The authors acknowledge the funding provided by the National Key R&D Program of China (no. 2017YFB1002900) and the European Research Council (ERC) under the European Union’s Horizon 2020 research and innovation programme (grant agreement no. 724306). L.H. acknowledge the support from the National Natural Science Foundation of China (no. 61775019) program, the Beijing Municipal Natural Science Foundation (no. 4172057), the Beijing Nova Program (no. Z171100001117047), the Fok YingTong Education Foundation of China (no. 161009) and the Young Elite Scientists Sponsorship Program by CAST (no. 2016QNRC001).
Author information
Authors and Affiliations
Contributions
L.H. and T.Z. proposed the idea, L.H. and R.Z. conducted pattern designs and numerical simulations, Q.W. and R.Z. conducted the hologram generation, B.S. and C.T. fabricated the samples, T.Z., L.H., R.Z., and B.S. performed the measurements, L.H., T.Z., R.Z., and B.S. prepared the manuscript. L.H., Y.W., and T.Z. supervised the overall project. All of the authors analyzed the data and discussed the results.
Corresponding authors
Ethics declarations
Conflict of interest
The authors declare that they have no conflict of interest.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Zhao, R., Sain, B., Wei, Q. et al. Multichannel vectorial holographic display and encryption. Light Sci Appl 7, 95 (2018). https://doi.org/10.1038/s4137701800910
Received:
Revised:
Accepted:
Published:
DOI: https://doi.org/10.1038/s4137701800910
Further reading

Pancharatnam–Berry phase reversal via oppositechiralitycoexisted superstructures
Light: Science & Applications (2022)

Tunable liquid crystal grating based holographic 3D display system with wide viewing angle and large size
Light: Science & Applications (2022)

Design of scalable metalens array for optical addressing
Frontiers of Optoelectronics (2022)

AllDielectric PhaseGradient Metasurface Performing HighEfficiency Anomalous Transmission in the NearInfrared Region
Nanoscale Research Letters (2021)

Multifunctional metasurfaces enabled by simultaneous and independent control of phase and amplitude for orthogonal polarization states
Light: Science & Applications (2021)